Text of NMB SPLICE-SLEEVE SYSTEM Grout Operation 2013.2.pdf · Seismic Reinforcement. SRC Structure. ......
NMB SPLICE-SLEEVE SYSTEM
SPLICE SLEEVE NORTH AMERICA, INC.
Mid-Rise Wall Precast
High-Rise Wall Precast
Precast Distribution Warehouse Precast Hospital
Precast Super High-Rise Residential
Seismic Reinforcement SRC Structure
Railroad RC Pile Box Culvert
Precast Elevated Bridge
Precast Railroad Viaduct
Nuclear Power Plant-IntakePower Plant-Turbine Tower
GROUTING OPERATION: ACCESSORIES & MATERIALS
SS Mortar® SS Mortar
Grout Pump Manual/Electric/Air Operated
Handy PumpUse as a backup in case of power outage
Grout Hose For grout pump
Stopper with Indicator (SWI） At Grout Outlet ports
Self-Sealing Valve (SSV)
At Grout Inlet ports
NozzleUse a nozzle to fit into Self-Sealing Valve
GROUT MIXING: TOOLS & EQUIPMENTITEM DESCRIPTION
Mixing BucketUse 5 gallon（19 liters）steel pail. Avoid using plastic bucket.
Measuring Pail For measuring 1 gallon (3.785 liters) of water
ScaleFor measuring the correct weight of water (use as an alternative)
Electric Drill (≥ 7 amp, 500-1300 RPM)
Mixing Paddle NMB paddle
Stopwatch Timing the required mixing time
Cutter To open SS Mortar
Portable Heater Use during winter as necessary
GROUT TESTING AND CUBE SPECIMENS: TOOLS & EQUIPMENT
Measuring Cup2 pint (0.95 liters). Use for pouring mixed grout into flow cylinder and cubic molds
Thermometer Measure temperature of air, water, and materials
Flow TableFor consistency test. 13.39” x 13.39” x 0.79” (340 x 340 x 20 mm)
Flow Cylinder 2” dia. x 4” high
Tape Measure To measure the diameter of the puddle for consistency test
Angle Adjuster For leveling the flow table as necessary
Leveler To check the leveling of flow table
Spatula/Cement KnifeFor removing excess grout during consistency and compressive strength tests
Tamper/Rubber Stick For tamping grout during compressive strength test
For tapping the mold during compressive strength test
2” Triple (Brass or Steel) Cube mold For assembling specimens for compressive strength test
Curing Box For curing specimens for compressive strength test
GROUT TESTING AND CUBE SPECIMENS: TOOLS & EQUIPMENT
Electric Power Supply
Equipment for saturation For sleeves and joint area
Air Compressor For passage inspection
Electrical Tape For securing grout tubes to the sleeve ports
Flashlight or Spotlight For passage and grouting inspection
Steel Rod For passage inspection and trouble-shooting
Sledge Hammer For passage inspection and trouble-shooting
WORKING MECHANISM OF SELF-SEALING VALVE
Inserts into PVC grout inlet tube. Flap opens while pumping, then closes when grouting stops, preventing backflow and
automatically sealing off the tube. Once grout stiffens, remove, clean and reuse. Saves time with plugs and prevents spills, waste and cleanup. It is recommended to start pumping slowly, especially while using self-sealing valve to avoid
clogging, which subsequently can be increased a little bit once a smooth grout flow isconfirmed.
WORKING MECHANISM OF STOPPER WITH INDICATOR
Ж It allows air and water to pass but when solid grout arrives it pushes the plunger back against the Stopper sealing off the tube automatically.
------------------------Ж Once grout
stiffens, remove - clean – reuse.
------------------------Ж Saves time,
catching cups & plugs, prevents spills & cleanup.
-------------------------Ж Combined with
the Self Sealing Valve, one person can grout.
Cheater-Beater Paint Paddle M525 Quik Mix M819
Jiffler Cross Blade NMB Paddle
ACCESSORIES FOR ERECTION
TO PREVENT BEDDING MORTAR GETTING INTO THE SPLICE SLEEVE
Coil Spring supports the Grout Washer
Heavy Duty Light Duty
A. • Work schedule
B. • Assign a number to each sleeve
C. • Inspection of sleeves through grout holes
D. • Procure electricity and water for mixing
E. • Procure required quantity of SS Mortar
F. • Grout sampling and testing for quality control
G. • Grouting operation of Sleeves
H. • Cleaning
I. • Record keeping
OUTLINE OF GROUTING OPERATION13
GROUTING METHODS FOR NMB SPLICE-SLEEVESPRE-GROUTING METHOD
The NMB Splice-Sleeve® is located at the top of the lower precast member to be spliced. The grout is gravity fed into the Splice-Sleeve and the upper member with projecting rebar is erected into position.
Pour or pump SS Mortar mixed into the wide end opening of the sleeves.
Rod with a small diameter wire to remove air in the grout.
Fill sleeves before placing bedding grout to prevent the grout accidentally dropped in the sleeves.
NOTE: remember that once filled, you have 40 minutes to set the precast. Best if precast is dry fitted to check all fits before filling.
GROUTING METHODS FOR NMB SPLICE-SLEEVES
The NMB Splice-Sleeve® is located in the bottom of the upper member with reinforcing bar projecting out of the top of the lower member. Following the placement of the upper member, grouting is achieve by low pressure pumping
PREPARE DAILY WORK SCHEDULE/MATERIALS16
INSPECTION OF SLEEVES PRIOR GROUTING
BLOW out loose materials inside sleeves
Water may also be used to flush out sleeves from top to bottom.
SS MORTAR REQUIREMENT FOR SLEEVES
SS Mortar® (Grout) manufactured by Splice Sleeve Japan, Ltd. is a special cementicious non-metallic filler grout developed for the NMB Splice-Sleeve System.
SS Mortar® (Grout) is packaged in 55-lbs (25-kg) moisture resistant bags.
Achieves: ≥14,000 psi Compressive Strength @ 28 day≥ 4,000 psi in less than 24 hours at 68oF (20oC)
Mixing water: 1 gallon
Mixing time: 2 ½ minutes minimum
REBAR Size Splice-Sleeve SS Mortar 5” PVC Tubes
+ 15% overage
U.S. Metric Model lb/sleeve Sleeves/Bag lb/sleeve Sleeves/Bag
#5 16 mm 5 U-X 0.94 58.8 1.26 40.2
#6 20 mm 6 U-X 1.31 42.0 1.76 30.7
#7 22 mm 7 U-X 2.06 26.7 2.65 20.7
#8 25 mm 8 U-X 2.70 20.4 3.46 16.2
#9 28 mm 9 U-X 3.20 17.2 3.95 13.8
#10 32 mm 10 U-X 4.01 13.7 4.94 11.2
#11 35 mm 11 U-X 5.01 11.0 6.02 9.1
#11 35 mm SNX11 4.91 11.2 6.99 9.3
#11 35 mm A11W 6.07 9.1 7.74 7.6
#14 40 mm 14 U-X 7.67 7.2 9.19 6.0
#18 57 mm 18 U 22.62 2.4 25.31 2.1
If pumping grout tubes add a little more - see example on chart. When “upsizing” add 20% for each rebar size.
An additional overage of 15% is recommended to provide for typicalwaste and field loss while continuously pumping large numbers of sleeves.
Store SS MORTAR in a cool dry place
50°F(10°C) - 80°F(27°C)
Cold Weather: Heat and keep above 40°F(4.4°C) inside the sleeves and after grouted. Best curing temperature at 60°F(15°C). Use Radian Heater, Electric Blanket, Hydronic Hose
Hot Weather: Use chilled mixing water to keep the mixed grout temp below 80°F(27°C)
Do not perform grouting when no shelter from rain or snow, under below 40°F, and/or harmful vibration/impacts are expected throughout curing time.
SS MORTAR GROUT PERFORMANCE DATA
SET TIME HR-MINFLOW GUIDE BLEEDING %
0.98 gal(3.7 liters)
41℉ (5℃) 9 hr. 31 min. 13 hr. 35 min. 6 1/4" (160 mm) 0.00%
68℉ (20℃) 4 hr. 18 min. 5 hr. 55 min. 6 5/8" (170 mm) 0.00%
86℉ (30℃) 2 hr. 23 min. 3 hr. 20 min. 6 1/2" (165 mm) 0.00%
SS Mortar® (Grout) - Fresh Mortar Test Results
Nonmetallic, SS Mortar® can be used in when the surrounding concrete and the sleeve temperature is between
35oF (2oC) up to 140oF (60oC).
Freezing grout before it is above 1,500 psi will deplete strength.
The grout itself should be mixed and pumped between50oF (10oC) and 95oF (35oC).
3,000 psi = 100% Fy = Specified Yield = 60ksi (ASTM Grade 60 rebar)4,000 psi = conservatively above Fy allowing for variation in cube versus sleeve curing temperatures.
Typically specified by EORs for removal of bracing and continued erection (typical structures)6,500 psi = 125% Fy (75ksi) = ACI Type 1 and AASHTO9,500 psi = 100% Specified Tensile (A615) * (90-ksi) = 150% Fy = ACI Type 2
*ASTM Grade 60, 615 rebar Fu = 90-ksi (706 rebar Fu = 80-ksi)
FRESHNESS” BAG LIFE OF NON-METALLIC SS MORTAR
CF 25: 13 - 06 - 25 = June 25, 2013
Nissco SS Mortar should be stored in moderate/cool and dry conditions.50oF – 80oF (10oC – 27oC)
It has a “freshness” bag life of one (1) year.
Bags have a date stamp on the top using letters for the year then month then numbers for the day .
MIXING OF SS MORTAR
SS Mortar® is a ready-to-use formulation requiring only the proper amount of water, which is suggested at 1.00 gal. = 3.8 liters per bag. The maximum water is 1.03 gal. = 3.9 liters. Do not use admixtures. The field consistency should be between 6.0" minimum and 9.25" maximum
Use a full bag unit for each batch. Do not use SS Mortar® (Grout) if the package is damaged. SS Mortar® (Grout) has a shelf life of approximately 12 months
Do not mix by hand.Do not add cement, sand, aggregate or admixtures.Do not add more water than specified, nor re-mix.Do not use partial bag( Use full bag each time)Do not use if the bag is damaged.Do not use a grout other than SS Mortar.Do not use SS Mortar beyond one year shelf life.Do not leave the mixed grout in the pump.
SOME DONT’S DURING MIXING OF SS MORTAR24
FLOW/CONSISTENCY MEASUREMENT OF SS MORTAR
Wipe the Flow Table surface with wet rag.
Pour SS Mortar into Flow Cylinder.
Level the surface at the rim with cement knife.
Lift Cylinder slowly vertically.
Measure the diameter in two ways. The diameter is be 6” – 9 ¼” (160mm - 230mm).
COUNTER MEASURES INCASE FLOW/CONSISTENCY TEST OF SS MORTAR IS NOT WITHIN RANGE
SS Mortar Grout Consistency/ Flow Test
Consistency less than 6”
Remix・Put all mixed grout back into the pail.
・Measure 0.1 or 0.2 liter of water accurately andadd to mixed grout.・Re-mix grout for 30-60 seconds.
Re-Measure the Consistency of SS Mortar
Fail: Dispose and Start Mixing a new batch of
Pass: Use Mixed Grout for Grouting of NMB
Consistency more than 9.25”
Discard the mix and start mixing a new batch of SS Mortar
Passed(Consistency within 6” and 9.25”)
Use Mixed Grout for Grouting of NMB Splice-Sleeves
Note:Dispose mixed grout in the following
① More than 30 minutes passed after thecompletion of the 1st mixing.
① The total amount of mixing waterexceeds 3.9 liter (1.03 gallon) per 25 kgbag.
PREPARATION/SAMPLING OF GROUT CUBE SPECIMENS
Grout is poured into the mold in two equal layers, each layerbeing tamped eight (8) times with the tamper and compactedby tapping the sides of the mold several times with a woodenhammer.
Remove excess grout with trowel and clean top edge of moldvery carefully.
Cover the molds with a heavy plate and wet cloth, then placethe specimens undisturbed for at least 24 hours in a curing box.
Strip the cubes following day, mark to identify on top trowelsurface and cure them in lime water for 28 days or until tested.
COMPRESSIVE STRENGTH TESTING OF GROUT CUBE SPECIMENS
2” (5 cm) Cube compressive test will be conducted according to ASTM C109-80Attention: Place the cube on its side other than the face levelled during
preparation. The cube must be placed at the dead center of compressive testingmachine
1. First, saturate the pump and grout hose with water to lubricate inside.
2. Pour the mixed grout into the pump hopper and operate the pump to push out the slurry from the hose.
3. After confirming a solid stream of grout coming out of the nozzle, stop pumping and insert the nozzle into the sleeve grout inlet.
4. Keep pumping the grout slowly until a solid flow of grout can be seen from the outlet hole.
5. Catch the overflow in a cup and seal the outlet with stopper.6. Then, withdraw the nozzle and seal the inlet hole with the
GROUTING OF NMB SPLICE-SLEEVES29
GROUTING OF NMB SPLICE-SLEEVES
Working Time: 40 minutes
A: Pump grout into sleeve though the inlet port continuously and slowly
B: Catch the overflow in a cup and seal the outlet hole with a rubber stopper.
C: Withdraw the nozzlefrom the inlet hole and sealit with a rubber stopper.
NO. ITEM TESTING /INSPECTION METHOD CRITERIA
1 Material inspection
Check for the Lot Number printed on the bag to confirm the bag life, which should be within one year period to the date of grouting
Make sure that SS Mortar did not expire the bag life of one year
2 Rain water seepage Visual inspection on SS Mortar Make sure that no rain water is inside the material
3 Sleeve temperature Measure the temperature with a thermometer Should be between 35 ～140℉ (2～60℃）
4 Location & quantity of sleeves Check the specification/drawings Make sure that the location and quantity
match the specification/drawings
5 Dowel embedment length Check for proper dowel embedment length
Make sure that the embedment length of dowel is as per the requirement in the User's Manual
6 Inside sleeve Visual inspection Make sure that sleeve inside is clean and free from loose materials
7 Sleeve passage
Check the sleeve by blowing out air through the ports or check for sound by tapping the port, for confirmation of a clear passage
Make sure that there is a clear passage from the inlet to outlet ports
CHECK-LIST: PRIOR GROUTING31
NO. ITEM TESTING /INSPECTION METHOD CRITERIA
8 Mixing water Confirm as per the User's Manual 1 gallon /55 lbs. bag (0.95～1.03 gallon/55 lbs. bag)
9 Mixing temperature Confirm as per the User's Manual 50～95℉ (10～35℃）
10 Mixing time Confirm as per the User's Manual 2-1/2 minutes
11 Grout working time Confirm as per the User's Manual Within 40 minutes
12 Consistency test Confirm as per the User's Manual The consistency measurement should fall in the range of 6" to 9-1/4".
13 Inspection at grouting (Pre- Grout) Confirm as per the User's Manual
Make sure that all the sleeves were totally filled with SS Mortar. Make sure that the bedding mortar does not get inside the sleeves
14 Inspection at grouting (Post- Grout) Confirm as per the User's Manual
Make sure that all the sleeves were totally grouted from inside and solid grout comes out from the outlet port
15 Inspection after grouting Confirm as per the User's Manual
Reconfirm that all sleeves and joint areas are completely grouted by using grouting report as a check sheet
CHECK-LIST: DURING & AFTER GROUTING32
GROUTING REPORT SAMPLE
REPORT OF GROUT WORK - INSPECTION SHEET
AmbientLocation Dry GroutDate of Grouting Mixing WaterDate of Inspection Grout as MixedReport by SS Mortar Lot No.Approved by Flow Measurement
NMb Sleeve Size Quantity Plan Grouted Balance MEMO
5U-X 10 10 10 0 OK
6U-X 12 12 10 2 Ports Missing
Inlet/outlet ports do not reach the surface
1. Check and mark the position of the ports according to the drawings.
2. Chip out the concrete at the marked positions to find the embedded ports.
3. Blow out the ports with the air compressors or water and confirm that there is a clear passage from the inlet to outlet port.
Due to omission of washers, the inlet port is clogged with bedding mortar from the joint
1. Insert a steel rod into the ports and hammer it to clear the port.
2. Repeat step 3 of Item 1.
Inlet and/or outlet port is clogged with concrete debris etc. or plastic Hole Seals (sealing caps)
For debris etc.: Insert a steel rod into the ports and hammer it to clear the port.
For Hole seals:1. Use a hooked rod to scrape seals out of the ports. 2. Repeat step 3 of Item 1.
Leakage during pumping of grout from the joint due to incomplete mortar bedding
1. Seal the joint with rags, polyurethane, mortar, etc.
2 Clean the inside of the sleeve with water. (Preferably high pressure).
3. Confirm a clear passage by blowing with air.
6. Clogging has occurred inside the sleeve such as at point marked during pumping operation
1. Clean the inside with high pressure water
2. After confirming a clear passage by blowing with air, start re-grouting at about half speed of the normal operation
7. Rebar is too close to the outlet port, restricting grout flow
1. Insert heavy punch into outlet grout tube and strike with sledge hammer to reduce restriction
OVERVIEW VIDEO OF GROUTING PROCESS
I 85 Bridge Construction using NMBs _ Please click on the link to watch the video